University of Groningen Synthesis and characterization of 2016. 3. 5.آ Luc Ubaghs 1, Bhaskar...
Embed Size (px)
Transcript of University of Groningen Synthesis and characterization of 2016. 3. 5.آ Luc Ubaghs 1, Bhaskar...
University of Groningen
Synthesis and characterization of alternating poly(amide urea)s and poly(amide urethane urethane)s from ε-caprolactam, diamines, and diphenyl carbonate or ethylene carbonate Ubaghs, Luc; Sharma, Bhaskar; Keul, Helmut; Höcker, Hartwig; Loontjens, Ton; Benthem, Rolf van Published in: E-Polymers
IMPORTANT NOTE: You are advised to consult the publisher's version (publisher's PDF) if you wish to cite from it. Please check the document version below.
Document Version Publisher's PDF, also known as Version of record
Publication date: 2003
Link to publication in University of Groningen/UMCG research database
Citation for published version (APA): Ubaghs, L., Sharma, B., Keul, H., Höcker, H., Loontjens, T., & Benthem, R. V. (2003). Synthesis and characterization of alternating poly(amide urea)s and poly(amide urethane urethane)s from ε-caprolactam, diamines, and diphenyl carbonate or ethylene carbonate. E-Polymers, (68), 1-16.
Copyright Other than for strictly personal use, it is not permitted to download or to forward/distribute the text or part of it without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license (like Creative Commons).
Take-down policy If you believe that this document breaches copyright please contact us providing details, and we will remove access to the work immediately and investigate your claim.
Downloaded from the University of Groningen/UMCG research database (Pure): http://www.rug.nl/research/portal. For technical reasons the number of authors shown on this cover page is limited to 10 maximum.
Download date: 18-06-2021
e-Polymers 2003, no. 068. ISSN 1618-7229
Synthesis and characterization of alternating poly(amide urea)s and poly(amide urethane urethane)s from ε-caprolactam, diamines, and diphenyl carbonate or ethylene carbonate Luc Ubaghs 1, Bhaskar Sharma 1, Helmut Keul 1 *, Hartwig Höcker 1 *, Ton Loontjens 2, Rolf van Benthem 2 1 Lehrstuhl für Textilchemie und Makromolekulare Chemie der Rheinisch- Westfälischen Technischen Hochschule Aachen, Worringerweg 1, 52056 Aachen, Germany; Fax +49 241 8022438; firstname.lastname@example.org 2 DSM Research, PO Box 18, 6160 MD Geleen, The Netherlands (Submitted: October 20, 2003; published: December 17, 2003)
Abstract: Alternating poly(amide urea)s from ε-caprolactam, diamines H2N-(CH2)x- NH2 (x = 2 - 4), and diphenyl carbonate were prepared in two steps. The micro- structure of the poly(amide urea)s, as determined by means of 1H NMR spectro- scopy, reveals a strictly alternating sequence of the building blocks. The molecular weights and polydispersities obtained were 7500 < Mn < 10 000 and 1.48 < Mw/Mn < 1.56, respectively. Thermal properties were determined by means of differential scanning calorimetry (DSC) (163.9°C < Tm < 197.2°C; 55.5°C < Tg (2nd heating) < 72.2°C), and thermogravimetric analysis (TGA). TGA shows a three-step decom- position at 200, 350, and 450°C, which was attributed to the cleavage of O-phenyl urethane end groups, as well as urea and amide linkages. These assignments were made by comparison with model compounds. Furthermore, alternating poly- (amide urethane urethane)s from ε-caprolactam, diamines, and ethylene carbonate were prepared in three steps. The microstructure of the poly(amide urethane urethane)s, as determined by means of 1H NMR spectroscopy, reveals imper- fections. The molecular weights and polydispersities obtained were 5400 < Mn < 17 000 and 2.08 < Mw/Mn < 2.99, respectively. Thermal properties were determined by means of DSC (155.9°C < Tm < 159.0°C; 35.5°C < Tg (2nd heating) < 39.0°C) and TGA. TGA shows a complex decomposition due to the formation of ethylene carbonate by cleavage of the urethane groups (at approx. 230°C) and formation of poly(amide urea)s. The newly formed poly(amide urea)s decompose in a similar way as the poly(amide urea)s.
Introduction Three important classes of polymers with carbon, oxygen, and nitrogen atoms in the main chain are polyamides, polyurethanes, and polyureas. Linear [m,n]-polyamides are prepared via polycondensation of an AA with a BB monomer, e.g., a diamine and a dicarboxylic acid. AB monomers, e.g., lactams, are used for the preparation of [n]-polyamides . Commercially manufactured polyurethanes are prepared from di- or polyfunctional hydroxy compounds and di- or polyfunctional isocyanates. Poly- urethanes but also urethane-containing copolymers are widely used to make foams,
fibres, elastomers, adhesives, and coatings [2–4]. The chemistry and technology of polyureas began in the 1960s, which is relatively late compared to polyamides and polyurethanes. Nowadays, polyureas are prepared from aliphatic, aromatic or hetero- cyclic polyamines (mainly diamines) with carbon dioxide, carbon oxysulfide, carbonic acid esters, phosgene, urea, urethanes, or isocyanates . In order to cover a wide range of properties, it is interesting to prepare polymers with different functional groups. The properties of these polymers are not only determined by the building blocks but also by the concentration and by the distribution – random or regular – of the functional groups. Excellent examples of this principle are the poly- (ester amide)s [6-17]. Due to hydrogen bonds between the amide groups, these materials have improved mechanical and thermal properties compared with poly- esters; the ester groups are mainly responsible for hydrolytical degradation. The aim of this work is to synthesize alternating poly(amide urea)s and alternating poly(amide urethane urethane)s by using ε-caprolactam, diamines, and diphenyl carbonate or ethylene carbonate. These polymers contain amide and urea or urethane groups thus combining the properties of three important classes of polymers with carbon, oxygen, and nitrogen in the main chain. Experimental part Materials ε-Caprolactam (BASF), 1,2-diaminoethane (BASF), 1,3-diaminopropane (BASF), 1,4- diaminobutane (67.5 wt.-% in water, DSM), diphenyl carbonate (Merck), ethylene carbonate (Acros Organics), and dibutyldimethoxytin (Bu2Sn(OMe)2, Aldrich) were used as received. Measurements 1H and 13C NMR spectra were recorded on a Bruker DPX-300 FT-NMR spectrometer at 300 and 75 MHz, respectively. Chloroform (CDCl3), dimethyl sulfoxide (DMSO-d6), formic acid (DCOOD), and trifluoroacetic acid (TFA-d1) were used as solvents, and tetramethylsilane (TMS) served as internal standard. Gel permeation chromatography (GPC) analyses were carried out using a high- pressure liquid chromatography pump (Bischoff HPLC pump 2200) and a refractive index detector (Waters 410). The eluting solvent was N,N-dimethylacetamide (DMAc) with 2.441 g/L LiCl. The flow rate was 0.8 mL/min. Four columns with MZ-DVB gel were applied: length of each column 300 mm, diameter 8 mm, diameter of gel particles 5 µm, nominal pore width 100 Å, 100 Å, 103 Å, 104 Å. Calibration was achieved using polystyrene standards of narrow molecular weight distribution from Polymer Standard Service, Mainz. Differential scanning calorimetric (DSC) analyses were performed with a Netzsch DSC 204 in nitrogen atmosphere with a heating rate of 10 K/min. Calibration was achieved using indium standard samples. Thermogravimetric analyses (TGA) were performed on a TG 209 with a TA-System- Controller TASC 414/2 from Netzsch. The measurements were performed in nitrogen atmosphere with a heating rate of 10 K/min.
Syntheses Amide-diamines 3a-c 6-Aminohexanoic acid 3-aminopropylamide 3b: ε-Caprolactam (9.09 g, 80.3 mmol), 1,3-diaminopropane (33.8 mL, 402 mmol), and water (13 mL) were heated in an autoclave at 200°C for 20 h while the pressure increased to 4.6 bar. After cooling, excess of 1,3-diaminopropane and water was removed in vacuum at 35°C and yellow oil was left. All amide-diamines 3a-c were prepared according to the same procedure (Tab. 1).
Tab. 1. Yield and NMR data of amide-diamines 3a-c
Poly(amide urea) 4a Amide-diamine 3a (1.73 g, 10.0 mmol) was added to diphenyl carbonate (2.14 g, 10.0 mmol) in a condensation flask. Polycondensation was performed at 100°C for 1 h at normal pressure and 2 h at reduced pressure (10-2 mbar) with removal of phenol by distillation. For purification, the polymer was dissolved in formic acid (10 mL) and precipitated in diethyl ether (100 mL). The product was isolated by filtration and dried in vacuum at 50°C. All poly(amide urea)s 4a-c were prepared according to the same procedure (Tab. 2 and Tab. 3).
Tab. 2. NMR data of the alternating poly(amide urea)s 4a-c
S = solvent, D = DMSO-d6 at 80°C, T = TFA-d1, F = DCOOD Tab. 3. Yield and molecular weight of the alternating poly(amide urea)s 4a-c
Compound Yield in % Mn Mw Mw/Mn
4a 67 10 000 16 000 1.56 4b 82 7500 11 000 1.48 4c 95 not soluble in DMAc at 80°C
α,ω-Diols 5a-c 5-[3-(2-Hydroxyethoxycarbonylamino)propylcarbamoyl]pentylcarbamic acid 2-hydro- xyethyl ester 5b: A solution of ethylene carbonate (3.12 g, 35.4 mmol) in ethylene glycol (22 mL) was added slowly to the amide-diamine 3b (2.17 g, 11.8 mol). After stirring for 23 h at room temperature, ethylene glycol was removed in vacuum (10-2 mbar) at 60°C to give a colourless wax (yield: 93%). All α,ω-diols 5a-c we